 
data_fr12-a 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H2 Ca Fe3 K0.50 Mg5 Na0.50 O24 Si5' 
_chemical_formula_weight          886.69 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mg'  'Mg'   0.0486   0.0363 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Si'  'Si'   0.0817   0.0704 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            ? 
_symmetry_space_group_name_H-M    ? 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y, -z' 
 'x+1/2, y+1/2, z' 
 '-x+1/2, y+1/2, -z' 
 '-x, -y, -z' 
 'x, -y, z' 
 '-x+1/2, -y+1/2, -z' 
 'x+1/2, -y+1/2, z' 
 
_cell_length_a                    9.806(2) 
_cell_length_b                    17.999(3) 
_cell_length_c                    5.296(2) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  105.43(2) 
_cell_angle_gamma                 90.00 
_cell_volume                      901.1(4) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        ? 
_exptl_crystal_colour             ? 
_exptl_crystal_size_max           ? 
_exptl_crystal_size_mid           ? 
_exptl_crystal_size_min           ? 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.268 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              874 
_exptl_absorpt_coefficient_mu     3.440 
_exptl_absorpt_correction_type    ? 
_exptl_absorpt_correction_T_min   ? 
_exptl_absorpt_correction_T_max   ? 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             3698 
_diffrn_reflns_av_R_equivalents   0.0550 
_diffrn_reflns_av_sigmaI/netI     0.0315 
_diffrn_reflns_limit_h_min        -9 
_diffrn_reflns_limit_h_max        9 
_diffrn_reflns_limit_k_min        -21 
_diffrn_reflns_limit_k_max        21 
_diffrn_reflns_limit_l_min        -7 
_diffrn_reflns_limit_l_max        7 
_diffrn_reflns_theta_min          3.99 
_diffrn_reflns_theta_max          28.29 
_reflns_number_total              555 
_reflns_number_gt                 428 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0313P)²+9.9171P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.0000(5) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          555 
_refine_ls_number_parameters      49 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0504 
_refine_ls_R_factor_gt            0.0382 
_refine_ls_wR_factor_ref          0.0941 
_refine_ls_wR_factor_gt           0.0895 
_refine_ls_goodness_of_fit_ref    1.080 
_refine_ls_restrained_S_all       1.080 
_refine_ls_shift/su_max           1.041 
_refine_ls_shift/su_mean          0.234 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
T1 Si 0.2849(2) 0.08527(8) 0.3041(3) 0.0093(4) Uiso 1 1 d . . . 
T2 Si 0.2912(2) 0.17274(8) 0.8102(3) 0.0074(4) Uiso 1 1 d . . . 
M1 Mg 0.0000 0.08006(8) 0.5000 0.0100(4) Uiso 0.50 2 d SP . . 
M11 Fe 0.0000 0.08006(8) 0.5000 0.0100(4) Uiso 0.50 2 d SP . . 
M2 Mg 0.0000 0.17691(11) 0.0000 0.0077(5) Uiso 0.80 2 d SP . . 
M22 Fe 0.0000 0.17691(11) 0.0000 0.0077(5) Uiso 0.20 2 d SP . . 
M3 Mg 0.0000 0.0000 0.0000 0.0082(6) Uiso 0.68 4 d SP . . 
M33 Fe 0.0000 0.0000 0.0000 0.0082(6) Uiso 0.32 4 d SP . . 
M4 Ca 0.0000 0.27852(16) 0.5000 0.0102(7) Uiso 0.89 2 d SP . . 
M42 Mg 0.0000 0.262(2) 0.5000 0.014(10) Uiso 0.11 2 d SP . . 
AM Na 0.0361(14) 0.5000 0.0674(13) 0.029(2) Uiso 0.53 2 d SP . . 
A2 K 0.0000 0.482(4) 0.0000 0.029(2) Uiso 0.05 2 d SP . . 
O1 O 0.1082(6) 0.08631(19) 0.2199(7) 0.0087(9) Uiso 1 1 d . . . 
O2 O 0.1184(6) 0.17031(19) 0.7275(7) 0.0102(9) Uiso 1 1 d . . . 
O3 O 0.1055(8) 0.0000 0.7165(10) 0.0123(12) Uiso 1 2 d S . . 
O4 O 0.3642(6) 0.2517(2) 0.7877(7) 0.0123(9) Uiso 1 1 d . . . 
O5 O 0.3523(6) 0.1403(2) 0.1109(7) 0.0133(9) Uiso 1 1 d . . . 
O6 O 0.3491(5) 0.1183(2) 0.6096(7) 0.0128(9) Uiso 1 1 d . . . 
O7 O 0.3460(8) 0.0000 0.2833(11) 0.0176(14) Uiso 1 2 d S . . 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
T1 O7 1.662(3) . ? 
T1 O1 1.670(6) . ? 
T1 O5 1.681(4) . ? 
T1 O6 1.681(4) . ? 
T1 M3 3.218(2) . ? 
T1 M4 3.221(3) 7_556 ? 
T1 M1 3.230(2) . ? 
T1 A2 3.21(3) 7 ? 
T1 AM 3.339(9) 7 ? 
T1 AM 3.411(11) 3_545 ? 
T1 A2 3.51(4) 3_545 ? 
T2 O4 1.609(4) . ? 
T2 O2 1.634(6) . ? 
T2 O5 1.652(4) 1_556 ? 
T2 O6 1.653(4) . ? 
T2 M4 3.0739(19) 7_556 ? 
T2 M42 3.173(14) 7_556 ? 
T2 M4 3.462(3) . ? 
T2 A2 3.44(6) 7_556 ? 
T2 AM 3.517(6) 7_556 ? 
T2 A2 3.99(6) 3_546 ? 
M1 O3 1.957(5) 5_556 ? 
M1 O3 1.957(5) . ? 
M1 O1 2.043(4) . ? 
M1 O1 2.043(4) 2_556 ? 
M1 O2 2.167(4) . ? 
M1 O2 2.167(4) 2_556 ? 
M1 M11 2.882(3) 5_556 ? 
M1 M1 2.882(3) 5_556 ? 
M1 M3 3.0147(12) . ? 
M1 M33 3.0147(12) 1_556 ? 
M1 M3 3.0147(12) 1_556 ? 
M2 O4 1.974(5) 7_556 ? 
M2 O4 1.974(5) 8_454 ? 
M2 O2 2.083(4) 2_556 ? 
M2 O2 2.083(4) 1_554 ? 
M2 O1 2.117(4) 2 ? 
M2 O1 2.117(4) . ? 
M2 M42 3.058(19) . ? 
M2 M42 3.058(19) 1_554 ? 
M2 M1 3.1703(16) 1_554 ? 
M2 M11 3.1703(16) 1_554 ? 
M3 O3 2.038(5) 5_556 ? 
M3 O3 2.038(5) 1_554 ? 
M3 O1 2.058(4) 5 ? 
M3 O1 2.058(4) . ? 
M3 O1 2.058(4) 6 ? 
M3 O1 2.058(4) 2 ? 
M3 M11 3.0147(12) 5 ? 
M3 M1 3.0147(12) 5 ? 
M3 M11 3.0147(12) 5_556 ? 
M3 M1 3.0147(12) 1_554 ? 
M4 O4 2.339(4) 8_455 ? 
M4 O4 2.339(4) 7_556 ? 
M4 O2 2.419(5) 2_556 ? 
M4 O2 2.419(5) . ? 
M4 O6 2.536(5) 7_556 ? 
M4 O6 2.536(5) 8_455 ? 
M4 O5 2.625(5) 7_556 ? 
M4 O5 2.625(5) 8_455 ? 
M4 T2 3.0739(19) 7_556 ? 
M4 T2 3.0739(19) 8_455 ? 
M42 O2 2.18(3) 2_556 ? 
M42 O2 2.18(3) . ? 
M42 O4 2.288(6) 7_556 ? 
M42 O4 2.288(6) 8_455 ? 
M42 M22 3.058(19) 1_556 ? 
M42 M2 3.058(19) 1_556 ? 
M42 T2 3.173(14) 7_556 ? 
M42 T2 3.173(14) 8_455 ? 
AM A2 0.54(4) . ? 
AM A2 0.54(4) 5_565 ? 
AM AM 0.86(2) 5_565 ? 
AM O7 2.432(13) 3_455 ? 
AM O7 2.435(11) 7 ? 
AM O6 2.775(7) 4_556 ? 
AM O6 2.775(7) 7_556 ? 
AM O5 3.004(7) 4 ? 
AM O5 3.004(7) 7 ? 
AM T1 3.339(9) 4 ? 
AM T1 3.339(9) 7 ? 
AM T1 3.411(11) 3_455 ? 
A2 AM 0.54(4) 5_565 ? 
A2 A2 0.66(14) 5_565 ? 
A2 O7 2.417(11) 7 ? 
A2 O7 2.417(11) 3_455 ? 
A2 O5 2.78(5) 8_455 ? 
A2 O5 2.78(5) 7 ? 
A2 O6 2.84(4) 8_454 ? 
A2 O6 2.84(4) 7_556 ? 
A2 T1 3.21(3) 7 ? 
A2 T1 3.21(3) 8_455 ? 
A2 O6 3.30(5) 4_556 ? 
O2 M22 2.083(4) 1_556 ? 
O2 M2 2.083(4) 1_556 ? 
O3 M11 1.957(5) 5_556 ? 
O3 M1 1.957(5) 5_556 ? 
O3 M33 2.038(5) 1_556 ? 
O3 M3 2.038(5) 1_556 ? 
O4 M22 1.974(5) 7_556 ? 
O4 M2 1.974(5) 7_556 ? 
O4 M42 2.288(6) 7_556 ? 
O4 M4 2.339(4) 7_556 ? 
O5 T2 1.652(4) 1_554 ? 
O5 M4 2.625(5) 7_556 ? 
O5 A2 2.78(5) 7 ? 
O5 AM 3.004(7) 7 ? 
O5 A2 3.32(6) 3_545 ? 
O6 M4 2.536(5) 7_556 ? 
O6 AM 2.775(7) 7_556 ? 
O6 A2 2.84(4) 7_556 ? 
O6 A2 3.30(5) 3_546 ? 
O7 T1 1.662(3) 6 ? 
O7 A2 2.417(11) 7 ? 
O7 A2 2.417(11) 3_545 ? 
O7 AM 2.432(13) 3_545 ? 
O7 AM 2.435(11) 7 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O7 T1 O1 111.1(3) . . ? 
O7 T1 O5 107.3(2) . . ? 
O1 T1 O5 112.3(2) . . ? 
O7 T1 O6 109.9(3) . . ? 
O1 T1 O6 110.5(2) . . ? 
O5 T1 O6 105.6(2) . . ? 
O7 T1 M3 78.9(3) . . ? 
O1 T1 M3 34.03(12) . . ? 
O5 T1 M3 113.97(18) . . ? 
O6 T1 M3 134.70(18) . . ? 
O7 T1 M4 120.5(3) . 7_556 ? 
O1 T1 M4 128.42(13) . 7_556 ? 
O5 T1 M4 54.35(15) . 7_556 ? 
O6 T1 M4 51.32(14) . 7_556 ? 
M3 T1 M4 158.61(7) . 7_556 ? 
O7 T1 M1 110.7(2) . . ? 
O1 T1 M1 33.03(12) . . ? 
O5 T1 M1 136.58(18) . . ? 
O6 T1 M1 80.55(17) . . ? 
M3 T1 M1 55.75(4) . . ? 
M4 T1 M1 117.84(5) 7_556 . ? 
O7 T1 A2 47.4(11) . 7 ? 
O1 T1 A2 130.1(4) . 7 ? 
O5 T1 A2 59.9(11) . 7 ? 
O6 T1 A2 119.2(3) . 7 ? 
M3 T1 A2 99.7(7) . 7 ? 
M4 T1 A2 89.2(10) 7_556 7 ? 
M1 T1 A2 152.9(10) . 7 ? 
O7 T1 AM 44.02(19) . 7 ? 
O1 T1 AM 121.3(2) . 7 ? 
O5 T1 AM 63.83(15) . 7 ? 
O6 T1 AM 127.5(3) . 7 ? 
M3 T1 AM 90.49(19) . 7 ? 
M4 T1 AM 97.91(17) 7_556 7 ? 
M1 T1 AM 144.23(17) . 7 ? 
A2 T1 AM 9.2(6) 7 7 ? 
O7 T1 AM 41.5(2) . 3_545 ? 
O1 T1 AM 134.9(2) . 3_545 ? 
O5 T1 AM 66.58(17) . 3_545 ? 
O6 T1 AM 113.0(2) . 3_545 ? 
M3 T1 AM 102.54(16) . 3_545 ? 
M4 T1 AM 89.18(15) 7_556 3_545 ? 
M1 T1 AM 151.14(12) . 3_545 ? 
A2 T1 AM 8.7(6) 7 3_545 ? 
AM T1 AM 14.6(3) 7 3_545 ? 
O7 T1 A2 37.6(9) . 3_545 ? 
O1 T1 A2 126.2(4) . 3_545 ? 
O5 T1 A2 69.7(10) . 3_545 ? 
O6 T1 A2 120.8(2) . 3_545 ? 
M3 T1 A2 93.7(6) . 3_545 ? 
M4 T1 A2 97.5(8) 7_556 3_545 ? 
M1 T1 A2 144.0(9) . 3_545 ? 
A2 T1 A2 10(2) 7 3_545 ? 
AM T1 A2 8.6(4) 7 3_545 ? 
AM T1 A2 8.8(5) 3_545 3_545 ? 
O4 T2 O2 117.0(2) . . ? 
O4 T2 O5 109.2(2) . 1_556 ? 
O2 T2 O5 109.4(2) . 1_556 ? 
O4 T2 O6 103.9(2) . . ? 
O2 T2 O6 108.7(2) . . ? 
O5 T2 O6 108.2(2) 1_556 . ? 
O4 T2 M4 48.40(15) . 7_556 ? 
O2 T2 M4 130.91(14) . 7_556 ? 
O5 T2 M4 119.6(2) 1_556 7_556 ? 
O6 T2 M4 55.55(16) . 7_556 ? 
O4 T2 M42 43.4(6) . 7_556 ? 
O2 T2 M42 129.6(2) . 7_556 ? 
O5 T2 M42 120.8(3) 1_556 7_556 ? 
O6 T2 M42 60.5(6) . 7_556 ? 
M4 T2 M42 5.2(6) 7_556 7_556 ? 
O4 T2 M4 78.8(2) . . ? 
O2 T2 M4 38.90(13) . . ? 
O5 T2 M4 133.89(18) 1_556 . ? 
O6 T2 M4 113.71(17) . . ? 
M4 T2 M4 99.91(4) 7_556 . ? 
M42 T2 M4 96.6(4) 7_556 . ? 
O4 T2 A2 119.6(7) . 7_556 ? 
O2 T2 A2 123.4(7) . 7_556 ? 
O5 T2 A2 53.0(2) 1_556 7_556 ? 
O6 T2 A2 55.2(2) . 7_556 ? 
M4 T2 A2 87.6(4) 7_556 7_556 ? 
M42 T2 A2 92.0(7) 7_556 7_556 ? 
M4 T2 A2 159.2(7) . 7_556 ? 
O4 T2 AM 126.3(3) . 7_556 ? 
O2 T2 AM 116.1(2) . 7_556 ? 
O5 T2 AM 58.47(17) 1_556 7_556 ? 
O6 T2 AM 50.47(18) . 7_556 ? 
M4 T2 AM 89.68(18) 7_556 7_556 ? 
M42 T2 AM 94.5(6) 7_556 7_556 ? 
M4 T2 AM 150.41(18) . 7_556 ? 
A2 T2 AM 8.8(6) 7_556 7_556 ? 
O4 T2 A2 124.8(5) . 3_546 ? 
O2 T2 A2 118.1(5) . 3_546 ? 
O5 T2 A2 54.8(2) 1_556 3_546 ? 
O6 T2 A2 53.86(18) . 3_546 ? 
M4 T2 A2 90.6(3) 7_556 3_546 ? 
M42 T2 A2 95.3(6) 7_556 3_546 ? 
M4 T2 A2 153.7(5) . 3_546 ? 
A2 T2 A2 5.6(12) 7_556 3_546 ? 
AM T2 A2 4.0(4) 7_556 3_546 ? 
O3 M1 O3 85.2(3) 5_556 . ? 
O3 M1 O1 84.89(19) 5_556 . ? 
O3 M1 O1 99.8(2) . . ? 
O3 M1 O1 99.8(2) 5_556 2_556 ? 
O3 M1 O1 84.89(19) . 2_556 ? 
O1 M1 O1 173.7(2) . 2_556 ? 
O3 M1 O2 177.98(16) 5_556 . ? 
O3 M1 O2 96.00(19) . . ? 
O1 M1 O2 93.29(16) . . ? 
O1 M1 O2 81.96(16) 2_556 . ? 
O3 M1 O2 96.00(19) 5_556 2_556 ? 
O3 M1 O2 177.98(16) . 2_556 ? 
O1 M1 O2 81.96(16) . 2_556 ? 
O1 M1 O2 93.29(16) 2_556 2_556 ? 
O2 M1 O2 82.9(2) . 2_556 ? 
O3 M1 M11 42.59(15) 5_556 5_556 ? 
O3 M1 M11 42.59(15) . 5_556 ? 
O1 M1 M11 93.15(10) . 5_556 ? 
O1 M1 M11 93.15(10) 2_556 5_556 ? 
O2 M1 M11 138.56(12) . 5_556 ? 
O2 M1 M11 138.56(12) 2_556 5_556 ? 
O3 M1 M1 42.59(15) 5_556 5_556 ? 
O3 M1 M1 42.59(15) . 5_556 ? 
O1 M1 M1 93.15(10) . 5_556 ? 
O1 M1 M1 93.15(10) 2_556 5_556 ? 
O2 M1 M1 138.56(12) . 5_556 ? 
O2 M1 M1 138.56(12) 2_556 5_556 ? 
M11 M1 M1 0.0 5_556 5_556 ? 
O3 M1 M3 42.02(16) 5_556 . ? 
O3 M1 M3 92.24(13) . . ? 
O1 M1 M3 42.89(12) . . ? 
O1 M1 M3 141.74(13) 2_556 . ? 
O2 M1 M3 136.17(10) . . ? 
O2 M1 M3 89.73(9) 2_556 . ? 
M11 M1 M3 61.45(3) 5_556 . ? 
M1 M1 M3 61.45(3) 5_556 . ? 
O3 M1 M33 92.24(13) 5_556 1_556 ? 
O3 M1 M33 42.02(16) . 1_556 ? 
O1 M1 M33 141.74(13) . 1_556 ? 
O1 M1 M33 42.89(12) 2_556 1_556 ? 
O2 M1 M33 89.73(9) . 1_556 ? 
O2 M1 M33 136.17(10) 2_556 1_556 ? 
M11 M1 M33 61.45(3) 5_556 1_556 ? 
M1 M1 M33 61.45(3) 5_556 1_556 ? 
M3 M1 M33 122.89(5) . 1_556 ? 
O3 M1 M3 92.24(13) 5_556 1_556 ? 
O3 M1 M3 42.02(16) . 1_556 ? 
O1 M1 M3 141.74(13) . 1_556 ? 
O1 M1 M3 42.89(12) 2_556 1_556 ? 
O2 M1 M3 89.73(9) . 1_556 ? 
O2 M1 M3 136.17(10) 2_556 1_556 ? 
M11 M1 M3 61.45(3) 5_556 1_556 ? 
M1 M1 M3 61.45(3) 5_556 1_556 ? 
M3 M1 M3 122.89(5) . 1_556 ? 
M33 M1 M3 0.0 1_556 1_556 ? 
O4 M2 O4 98.7(3) 7_556 8_454 ? 
O4 M2 O2 93.36(16) 7_556 2_556 ? 
O4 M2 O2 90.90(17) 8_454 2_556 ? 
O4 M2 O2 90.90(17) 7_556 1_554 ? 
O4 M2 O2 93.36(16) 8_454 1_554 ? 
O2 M2 O2 173.5(2) 2_556 1_554 ? 
O4 M2 O1 168.10(19) 7_556 2 ? 
O4 M2 O1 91.42(18) 8_454 2 ? 
O2 M2 O1 92.70(16) 2_556 2 ? 
O2 M2 O1 82.24(16) 1_554 2 ? 
O4 M2 O1 91.42(18) 7_556 . ? 
O4 M2 O1 168.10(19) 8_454 . ? 
O2 M2 O1 82.24(16) 2_556 . ? 
O2 M2 O1 92.70(16) 1_554 . ? 
O1 M2 O1 79.3(2) 2 . ? 
O4 M2 M42 48.4(3) 7_556 . ? 
O4 M2 M42 90.7(5) 8_454 . ? 
O2 M2 M42 45.6(4) 2_556 . ? 
O2 M2 M42 139.2(4) 1_554 . ? 
O1 M2 M42 138.2(4) 2 . ? 
O1 M2 M42 91.4(5) . . ? 
O4 M2 M42 90.7(5) 7_556 1_554 ? 
O4 M2 M42 48.4(3) 8_454 1_554 ? 
O2 M2 M42 139.2(4) 2_556 1_554 ? 
O2 M2 M42 45.6(4) 1_554 1_554 ? 
O1 M2 M42 91.4(5) 2 1_554 ? 
O1 M2 M42 138.2(4) . 1_554 ? 
M42 M2 M42 120.0(12) . 1_554 ? 
O4 M2 M1 133.17(12) 7_556 1_554 ? 
O4 M2 M1 91.85(10) 8_454 1_554 ? 
O2 M2 M1 132.17(13) 2_556 1_554 ? 
O2 M2 M1 42.77(12) 1_554 1_554 ? 
O1 M2 M1 39.50(10) 2 1_554 ? 
O1 M2 M1 85.68(11) . 1_554 ? 
M42 M2 M1 176.6(6) . 1_554 ? 
M42 M2 M1 63.4(6) 1_554 1_554 ? 
O4 M2 M11 133.17(12) 7_556 1_554 ? 
O4 M2 M11 91.85(10) 8_454 1_554 ? 
O2 M2 M11 132.17(13) 2_556 1_554 ? 
O2 M2 M11 42.77(12) 1_554 1_554 ? 
O1 M2 M11 39.50(10) 2 1_554 ? 
O1 M2 M11 85.68(11) . 1_554 ? 
M42 M2 M11 176.6(6) . 1_554 ? 
M42 M2 M11 63.4(6) 1_554 1_554 ? 
M1 M2 M11 0.00(5) 1_554 1_554 ? 
O4 M2 M1 91.85(10) 7_556 . ? 
O4 M2 M1 133.17(12) 8_454 . ? 
O2 M2 M1 42.77(12) 2_556 . ? 
O2 M2 M1 132.17(13) 1_554 . ? 
O1 M2 M1 85.68(11) 2 . ? 
O1 M2 M1 39.50(10) . . ? 
M42 M2 M1 63.4(6) . . ? 
M42 M2 M1 176.6(6) 1_554 . ? 
M1 M2 M1 113.29(8) 1_554 . ? 
M11 M2 M1 113.29(8) 1_554 . ? 
O3 M3 O3 180.0(3) 5_556 1_554 ? 
O3 M3 O1 97.50(16) 5_556 5 ? 
O3 M3 O1 82.50(16) 1_554 5 ? 
O3 M3 O1 82.50(16) 5_556 . ? 
O3 M3 O1 97.50(16) 1_554 . ? 
O1 M3 O1 180.0(2) 5 . ? 
O3 M3 O1 82.50(16) 5_556 6 ? 
O3 M3 O1 97.50(16) 1_554 6 ? 
O1 M3 O1 82.0(2) 5 6 ? 
O1 M3 O1 98.0(2) . 6 ? 
O3 M3 O1 97.50(16) 5_556 2 ? 
O3 M3 O1 82.50(16) 1_554 2 ? 
O1 M3 O1 98.0(2) 5 2 ? 
O1 M3 O1 82.0(2) . 2 ? 
O1 M3 O1 180.0(3) 6 2 ? 
O3 M3 M1 40.01(13) 5_556 . ? 
O3 M3 M1 139.99(13) 1_554 . ? 
O1 M3 M1 137.50(10) 5 . ? 
O1 M3 M1 42.50(10) . . ? 
O1 M3 M1 89.09(10) 6 . ? 
O1 M3 M1 90.91(10) 2 . ? 
O3 M3 M11 139.99(13) 5_556 5 ? 
O3 M3 M11 40.01(13) 1_554 5 ? 
O1 M3 M11 42.50(10) 5 5 ? 
O1 M3 M11 137.50(10) . 5 ? 
O1 M3 M11 90.91(10) 6 5 ? 
O1 M3 M11 89.09(10) 2 5 ? 
M1 M3 M11 180.00(5) . 5 ? 
O3 M3 M1 139.99(13) 5_556 5 ? 
O3 M3 M1 40.01(13) 1_554 5 ? 
O1 M3 M1 42.50(10) 5 5 ? 
O1 M3 M1 137.50(10) . 5 ? 
O1 M3 M1 90.91(10) 6 5 ? 
O1 M3 M1 89.09(10) 2 5 ? 
M1 M3 M1 180.00(5) . 5 ? 
M11 M3 M1 0.00(5) 5 5 ? 
O3 M3 M11 40.01(13) 5_556 5_556 ? 
O3 M3 M11 139.99(13) 1_554 5_556 ? 
O1 M3 M11 90.91(10) 5 5_556 ? 
O1 M3 M11 89.09(10) . 5_556 ? 
O1 M3 M11 42.50(10) 6 5_556 ? 
O1 M3 M11 137.50(10) 2 5_556 ? 
M1 M3 M11 57.11(5) . 5_556 ? 
M11 M3 M11 122.89(5) 5 5_556 ? 
M1 M3 M11 122.89(5) 5 5_556 ? 
O3 M3 M1 139.99(13) 5_556 1_554 ? 
O3 M3 M1 40.01(13) 1_554 1_554 ? 
O1 M3 M1 89.09(10) 5 1_554 ? 
O1 M3 M1 90.91(10) . 1_554 ? 
O1 M3 M1 137.50(10) 6 1_554 ? 
O1 M3 M1 42.50(10) 2 1_554 ? 
M1 M3 M1 122.89(5) . 1_554 ? 
M11 M3 M1 57.11(5) 5 1_554 ? 
M1 M3 M1 57.11(5) 5 1_554 ? 
M11 M3 M1 180.00(5) 5_556 1_554 ? 
O4 M4 O4 153.1(2) 8_455 7_556 ? 
O4 M4 O2 81.73(15) 8_455 2_556 ? 
O4 M4 O2 76.69(15) 7_556 2_556 ? 
O4 M4 O2 76.69(15) 8_455 . ? 
O4 M4 O2 81.73(15) 7_556 . ? 
O2 M4 O2 72.7(2) 2_556 . ? 
O4 M4 O6 141.92(16) 8_455 7_556 ? 
O4 M4 O6 63.45(13) 7_556 7_556 ? 
O2 M4 O6 135.06(11) 2_556 7_556 ? 
O2 M4 O6 118.14(16) . 7_556 ? 
O4 M4 O6 63.45(13) 8_455 8_455 ? 
O4 M4 O6 141.92(16) 7_556 8_455 ? 
O2 M4 O6 118.14(16) 2_556 8_455 ? 
O2 M4 O6 135.06(11) . 8_455 ? 
O6 M4 O6 85.8(2) 7_556 8_455 ? 
O4 M4 O5 84.78(14) 8_455 7_556 ? 
O4 M4 O5 110.46(15) 7_556 7_556 ? 
O2 M4 O5 158.55(15) 2_556 7_556 ? 
O2 M4 O5 88.02(14) . 7_556 ? 
O6 M4 O5 62.52(13) 7_556 7_556 ? 
O6 M4 O5 69.30(16) 8_455 7_556 ? 
O4 M4 O5 110.46(15) 8_455 8_455 ? 
O4 M4 O5 84.78(14) 7_556 8_455 ? 
O2 M4 O5 88.02(14) 2_556 8_455 ? 
O2 M4 O5 158.55(15) . 8_455 ? 
O6 M4 O5 69.30(16) 7_556 8_455 ? 
O6 M4 O5 62.52(13) 8_455 8_455 ? 
O5 M4 O5 112.4(2) 7_556 8_455 ? 
O4 M4 T2 171.93(13) 8_455 7_556 ? 
O4 M4 T2 30.96(10) 7_556 7_556 ? 
O2 M4 T2 105.28(10) 2_556 7_556 ? 
O2 M4 T2 101.31(11) . 7_556 ? 
O6 M4 T2 32.51(9) 7_556 7_556 ? 
O6 M4 T2 115.17(13) 8_455 7_556 ? 
O5 M4 T2 87.35(11) 7_556 7_556 ? 
O5 M4 T2 74.25(11) 8_455 7_556 ? 
O4 M4 T2 30.96(10) 8_455 8_455 ? 
O4 M4 T2 171.93(13) 7_556 8_455 ? 
O2 M4 T2 101.31(11) 2_556 8_455 ? 
O2 M4 T2 105.28(10) . 8_455 ? 
O6 M4 T2 115.17(13) 7_556 8_455 ? 
O6 M4 T2 32.51(9) 8_455 8_455 ? 
O5 M4 T2 74.25(11) 7_556 8_455 ? 
O5 M4 T2 87.35(11) 8_455 8_455 ? 
T2 M4 T2 146.83(12) 7_556 8_455 ? 
O4 M4 M2 121.91(13) 8_455 . ? 
O4 M4 M2 37.57(12) 7_556 . ? 
O2 M4 M2 40.33(9) 2_556 . ? 
O2 M4 M2 81.20(11) . . ? 
O6 M4 M2 95.75(8) 7_556 . ? 
O6 M4 M2 137.07(10) 8_455 . ? 
O5 M4 M2 147.28(10) 7_556 . ? 
O5 M4 M2 77.94(9) 8_455 . ? 
T2 M4 M2 64.95(4) 7_556 . ? 
T2 M4 M2 138.40(5) 8_455 . ? 
O2 M42 O2 82.1(13) 2_556 . ? 
O2 M42 O4 82.6(7) 2_556 7_556 ? 
O2 M42 O4 88.2(8) . 7_556 ? 
O2 M42 O4 88.2(8) 2_556 8_455 ? 
O2 M42 O4 82.6(7) . 8_455 ? 
O4 M42 O4 167.8(19) 7_556 8_455 ? 
O2 M42 M2 42.9(3) 2_556 . ? 
O2 M42 M2 88.7(10) . . ? 
O4 M42 M2 40.2(3) 7_556 . ? 
O4 M42 M2 131.1(11) 8_455 . ? 
O2 M42 M22 88.7(10) 2_556 1_556 ? 
O2 M42 M22 42.9(3) . 1_556 ? 
O4 M42 M22 131.1(11) 7_556 1_556 ? 
O4 M42 M22 40.2(3) 8_455 1_556 ? 
M2 M42 M22 120.0(12) . 1_556 ? 
O2 M42 M2 88.7(10) 2_556 1_556 ? 
O2 M42 M2 42.9(3) . 1_556 ? 
O4 M42 M2 131.1(11) 7_556 1_556 ? 
O4 M42 M2 40.2(3) 8_455 1_556 ? 
M2 M42 M2 120.0(12) . 1_556 ? 
M22 M42 M2 0.00(6) 1_556 1_556 ? 
O2 M42 T2 108.4(3) 2_556 7_556 ? 
O2 M42 T2 104.1(3) . 7_556 ? 
O4 M42 T2 28.9(3) 7_556 7_556 ? 
O4 M42 T2 162.7(14) 8_455 7_556 ? 
M2 M42 T2 65.70(6) . 7_556 ? 
M22 M42 T2 141.5(3) 1_556 7_556 ? 
M2 M42 T2 141.5(3) 1_556 7_556 ? 
O2 M42 T2 104.1(3) 2_556 8_455 ? 
O2 M42 T2 108.4(3) . 8_455 ? 
O4 M42 T2 162.7(14) 7_556 8_455 ? 
O4 M42 T2 28.9(3) 8_455 8_455 ? 
M2 M42 T2 141.5(3) . 8_455 ? 
M22 M42 T2 65.70(6) 1_556 8_455 ? 
M2 M42 T2 65.70(6) 1_556 8_455 ? 
T2 M42 T2 136.4(13) 7_556 8_455 ? 
O2 M42 M1 41.0(7) 2_556 . ? 
O2 M42 M1 41.0(7) . . ? 
O4 M42 M1 83.9(10) 7_556 . ? 
O4 M42 M1 83.9(10) 8_455 . ? 
M2 M42 M1 60.0(6) . . ? 
M22 M42 M1 60.0(6) 1_556 . ? 
M2 M42 M1 60.0(6) 1_556 . ? 
T2 M42 M1 111.8(6) 7_556 . ? 
T2 M42 M1 111.8(6) 8_455 . ? 
A2 AM A2 75(10) . 5_565 ? 
A2 AM AM 37(6) . 5_565 ? 
A2 AM AM 37(6) 5_565 5_565 ? 
A2 AM O7 82.1(17) . 3_455 ? 
A2 AM O7 82.1(17) 5_565 3_455 ? 
AM AM O7 80.0(15) 5_565 3_455 ? 
A2 AM O7 81.8(9) . 7 ? 
A2 AM O7 81.8(9) 5_565 7 ? 
AM AM O7 79.6(12) 5_565 7 ? 
O7 AM O7 159.6(5) 3_455 7 ? 
A2 AM O6 163(6) . 4_556 ? 
A2 AM O6 92(6) 5_565 4_556 ? 
AM AM O6 128.3(4) 5_565 4_556 ? 
O7 AM O6 86.9(2) 3_455 4_556 ? 
O7 AM O6 105.8(4) 7 4_556 ? 
A2 AM O6 92(6) . 7_556 ? 
A2 AM O6 163(6) 5_565 7_556 ? 
AM AM O6 128.3(4) 5_565 7_556 ? 
O7 AM O6 86.9(2) 3_455 7_556 ? 
O7 AM O6 105.8(4) 7 7_556 ? 
O6 AM O6 100.2(3) 4_556 7_556 ? 
A2 AM O5 122(5) . 4 ? 
A2 AM O5 61(5) 5_565 4 ? 
AM AM O5 91.6(6) 5_565 4 ? 
O7 AM O5 122.5(2) 3_455 4 ? 
O7 AM O5 58.22(17) 7 4 ? 
O6 AM O5 55.01(14) 4_556 4 ? 
O6 AM O5 135.8(5) 7_556 4 ? 
A2 AM O5 61(5) . 7 ? 
A2 AM O5 122(5) 5_565 7 ? 
AM AM O5 91.6(6) 5_565 7 ? 
O7 AM O5 122.5(2) 3_455 7 ? 
O7 AM O5 58.22(17) 7 7 ? 
O6 AM O5 135.8(5) 4_556 7 ? 
O6 AM O5 55.01(14) 7_556 7 ? 
O5 AM O5 114.5(4) 4 7 ? 
A2 AM T1 104(2) . 4 ? 
A2 AM T1 72(3) 5_565 4 ? 
AM AM T1 87.5(11) 5_565 4 ? 
O7 AM T1 150.0(2) 3_455 4 ? 
O7 AM T1 28.32(10) 7 4 ? 
O6 AM T1 79.6(2) 4_556 4 ? 
O6 AM T1 121.7(4) 7_556 4 ? 
O5 AM T1 30.15(11) 4 4 ? 
O5 AM T1 84.7(3) 7 4 ? 
A2 AM T1 72(3) . 7 ? 
A2 AM T1 104(2) 5_565 7 ? 
AM AM T1 87.5(11) 5_565 7 ? 
O7 AM T1 150.0(2) 3_455 7 ? 
O7 AM T1 28.32(10) 7 7 ? 
O6 AM T1 121.7(4) 4_556 7 ? 
O6 AM T1 79.6(2) 7_556 7 ? 
O5 AM T1 84.7(3) 4 7 ? 
O5 AM T1 30.15(11) 7 7 ? 
T1 AM T1 54.73(16) 4 7 ? 
A2 AM T1 96(4) . 3_455 ? 
A2 AM T1 63.9(14) 5_565 3_455 ? 
AM AM T1 77.9(13) 5_565 3_455 ? 
O7 AM T1 26.96(10) 3_455 3_455 ? 
O7 AM T1 144.7(3) 7 3_455 ? 
O6 AM T1 69.06(17) 4_556 3_455 ? 
O6 AM T1 109.4(3) 7_556 3_455 ? 
O5 AM T1 95.53(14) 4 3_455 ? 
O5 AM T1 148.6(3) 7 3_455 ? 
T1 AM T1 123.65(10) 4 3_455 ? 
T1 AM T1 165.4(3) 7 3_455 ? 
AM A2 AM 105(10) . 5_565 ? 
AM A2 A2 53(6) . 5_565 ? 
AM A2 A2 53(6) 5_565 5_565 ? 
AM A2 O7 85.4(15) . 7 ? 
AM A2 O7 85(2) 5_565 7 ? 
A2 A2 O7 82.2(16) 5_565 7 ? 
AM A2 O7 85(2) . 3_455 ? 
AM A2 O7 85.4(15) 5_565 3_455 ? 
A2 A2 O7 82.2(16) 5_565 3_455 ? 
O7 A2 O7 164(3) 7 3_455 ? 
AM A2 O5 129(4) . 8_455 ? 
AM A2 O5 109(5) 5_565 8_455 ? 
A2 A2 O5 142.2(9) 5_565 8_455 ? 
O7 A2 O5 133(2) 7 8_455 ? 
O7 A2 O5 61.9(8) 3_455 8_455 ? 
AM A2 O5 109(5) . 7 ? 
AM A2 O5 129(4) 5_565 7 ? 
A2 A2 O5 142.2(9) 5_565 7 ? 
O7 A2 O5 61.9(8) 7 7 ? 
O7 A2 O5 133(2) 3_455 7 ? 
O5 A2 O5 75.5(18) 8_455 7 ? 
AM A2 O6 170(3) . 8_454 ? 
AM A2 O6 77(5) 5_565 8_454 ? 
A2 A2 O6 129.3(11) 5_565 8_454 ? 
O7 A2 O6 85.7(8) 7 8_454 ? 
O7 A2 O6 104.3(11) 3_455 8_454 ? 
O5 A2 O6 56.8(11) 8_455 8_454 ? 
O5 A2 O6 62.9(12) 7 8_454 ? 
AM A2 O6 77(5) . 7_556 ? 
AM A2 O6 170(3) 5_565 7_556 ? 
A2 A2 O6 129.3(11) 5_565 7_556 ? 
O7 A2 O6 104.3(11) 7 7_556 ? 
O7 A2 O6 85.7(8) 3_455 7_556 ? 
O5 A2 O6 62.9(12) 8_455 7_556 ? 
O5 A2 O6 56.8(11) 7 7_556 ? 
O6 A2 O6 101(2) 8_454 7_556 ? 
AM A2 T1 99(2) . 7 ? 
AM A2 T1 107.4(10) 5_565 7 ? 
A2 A2 T1 112.1(11) 5_565 7 ? 
O7 A2 T1 30.4(5) 7 7 ? 
O7 A2 T1 165(3) 3_455 7 ? 
O5 A2 T1 105(2) 8_455 7 ? 
O5 A2 T1 31.6(3) 7 7 ? 
O6 A2 T1 71.4(9) 8_454 7 ? 
O6 A2 T1 80.9(11) 7_556 7 ? 
AM A2 T1 107.4(10) . 8_455 ? 
AM A2 T1 99(2) 5_565 8_455 ? 
A2 A2 T1 112.1(11) 5_565 8_455 ? 
O7 A2 T1 165(3) 7 8_455 ? 
O7 A2 T1 30.4(5) 3_455 8_455 ? 
O5 A2 T1 31.6(3) 8_455 8_455 ? 
O5 A2 T1 105(2) 7 8_455 ? 
O6 A2 T1 80.9(11) 8_454 8_455 ? 
O6 A2 T1 71.4(9) 7_556 8_455 ? 
T1 A2 T1 136(2) 7 8_455 ? 
AM A2 O6 14(5) . 4_556 ? 
AM A2 O6 94(7) 5_565 4_556 ? 
A2 A2 O6 41.8(8) 5_565 4_556 ? 
O7 A2 O6 92.2(14) 7 4_556 ? 
O7 A2 O6 76.1(12) 3_455 4_556 ? 
O5 A2 O6 128.96(11) 8_455 4_556 ? 
O5 A2 O6 123.34(13) 7 4_556 ? 
O6 A2 O6 171.1(19) 8_454 4_556 ? 
O6 A2 O6 87.5(3) 7_556 4_556 ? 
T1 A2 O6 110.4(7) 7 4_556 ? 
T1 A2 O6 102.2(6) 8_455 4_556 ? 
T1 O1 M1 120.5(2) . . ? 
T1 O1 M3 119.0(2) . . ? 
M1 O1 M3 94.61(18) . . ? 
T1 O1 M2 119.2(2) . . ? 
M1 O1 M2 99.25(19) . . ? 
M3 O1 M2 99.4(2) . . ? 
T2 O2 M22 122.8(2) . 1_556 ? 
T2 O2 M2 122.8(2) . 1_556 ? 
M22 O2 M2 0.0 1_556 1_556 ? 
T2 O2 M42 119.3(5) . . ? 
M22 O2 M42 91.51(19) 1_556 . ? 
M2 O2 M42 91.51(19) 1_556 . ? 
T2 O2 M1 122.2(2) . . ? 
M22 O2 M1 96.47(19) 1_556 . ? 
M2 O2 M1 96.47(19) 1_556 . ? 
M42 O2 M1 97.5(7) . . ? 
T2 O2 M4 115.99(19) . . ? 
M22 O2 M4 90.96(17) 1_556 . ? 
M2 O2 M4 90.96(17) 1_556 . ? 
M42 O2 M4 4.7(7) . . ? 
M1 O2 M4 102.21(19) . . ? 
M11 O3 M1 0.00(6) 5_556 5_556 ? 
M11 O3 M1 94.8(3) 5_556 . ? 
M1 O3 M1 94.8(3) 5_556 . ? 
M11 O3 M33 98.0(2) 5_556 1_556 ? 
M1 O3 M33 98.0(2) 5_556 1_556 ? 
M1 O3 M33 98.0(2) . 1_556 ? 
M11 O3 M3 98.0(2) 5_556 1_556 ? 
M1 O3 M3 98.0(2) 5_556 1_556 ? 
M1 O3 M3 98.0(2) . 1_556 ? 
M33 O3 M3 0.0 1_556 1_556 ? 
T2 O4 M22 141.1(2) . 7_556 ? 
T2 O4 M2 141.1(2) . 7_556 ? 
M22 O4 M2 0.00(8) 7_556 7_556 ? 
T2 O4 M42 107.7(9) . 7_556 ? 
M22 O4 M42 91.4(6) 7_556 7_556 ? 
M2 O4 M42 91.4(6) 7_556 7_556 ? 
T2 O4 M4 100.64(19) . 7_556 ? 
M22 O4 M4 96.2(2) 7_556 7_556 ? 
M2 O4 M4 96.2(2) 7_556 7_556 ? 
M42 O4 M4 7.3(10) 7_556 7_556 ? 
T2 O5 T1 134.0(3) 1_554 . ? 
T2 O5 M4 122.9(2) 1_554 7_556 ? 
T1 O5 M4 94.29(17) . 7_556 ? 
T2 O5 A2 98.7(4) 1_554 7 ? 
T1 O5 A2 88.5(8) . 7 ? 
M4 O5 A2 113.3(4) 7_556 7 ? 
T2 O5 AM 93.6(2) 1_554 7 ? 
T1 O5 AM 86.0(2) . 7 ? 
M4 O5 AM 122.9(3) 7_556 7 ? 
A2 O5 AM 9.8(4) 7 7 ? 
T2 O5 A2 101.3(3) 1_554 3_545 ? 
T1 O5 A2 82.0(6) . 3_545 ? 
M4 O5 A2 116.2(3) 7_556 3_545 ? 
A2 O5 A2 7.0(15) 7 3_545 ? 
AM O5 A2 7.93(13) 7 3_545 ? 
T2 O6 T1 136.3(3) . . ? 
T2 O6 M4 91.94(18) . 7_556 ? 
T1 O6 M4 97.51(16) . 7_556 ? 
T2 O6 AM 102.2(2) . 7_556 ? 
T1 O6 AM 108.0(2) . 7_556 ? 
M4 O6 AM 122.5(3) 7_556 7_556 ? 
T2 O6 A2 96.3(8) . 7_556 ? 
T1 O6 A2 117.7(10) . 7_556 ? 
M4 O6 A2 114.1(8) 7_556 7_556 ? 
AM O6 A2 11.0(10) 7_556 7_556 ? 
T2 O6 A2 102.3(6) . 3_546 ? 
T1 O6 A2 109.3(8) . 3_546 ? 
M4 O6 A2 119.8(5) 7_556 3_546 ? 
AM O6 A2 2.7(8) 7_556 3_546 ? 
A2 O6 A2 8.9(19) 7_556 3_546 ? 
T1 O7 T1 134.8(5) 6 . ? 
T1 O7 A2 117.6(16) 6 7 ? 
T1 O7 A2 102.2(16) . 7 ? 
T1 O7 A2 102.2(16) 6 3_545 ? 
T1 O7 A2 117.6(16) . 3_545 ? 
A2 O7 A2 16(3) 7 3_545 ? 
T1 O7 AM 111.5(2) 6 3_545 ? 
T1 O7 AM 111.5(2) . 3_545 ? 
A2 O7 AM 12.8(9) 7 3_545 ? 
A2 O7 AM 12.8(9) 3_545 3_545 ? 
T1 O7 AM 107.67(19) 6 7 ? 
T1 O7 AM 107.67(19) . 7 ? 
A2 O7 AM 12.8(9) 7 7 ? 
A2 O7 AM 12.8(9) 3_545 7 ? 
AM O7 AM 20.4(5) 3_545 7 ? 
 
_diffrn_measured_fraction_theta_max    0.480 
_diffrn_reflns_theta_full              28.29 
_diffrn_measured_fraction_theta_full   0.480 
_refine_diff_density_max    0.650 
_refine_diff_density_min   -0.877 
_refine_diff_density_rms    0.118 
